received: 23 March 2016 accepted: 20 May 2016 Published: 13 June 2016
Topological states and phase transitions in Sb2Te3-GeTe multilayers Thuy-Anh Nguyen1, Dirk Backes1, Angadjit Singh1, Rhodri Mansell1, Crispin Barnes1, David A. Ritchie1, Gregor Mussler2, Martin Lanius2, Detlev Grützmacher2 & Vijay Narayan1 Topological insulators (TIs) are bulk insulators with exotic ‘topologically protected’ surface conducting modes. It has recently been pointed out that when stacked together, interactions between surface modes can induce diverse phases including the TI, Dirac semimetal, and Weyl semimetal. However, currently a full experimental understanding of the conditions under which topological modes interact is lacking. Here, working with multilayers of the TI Sb2Te3 and the band insulator GeTe, we provide experimental evidence of multiple topological modes in a single Sb2Te3-GeTe-Sb2Te3 structure. Furthermore, we show that reducing the thickness of the GeTe layer induces a phase transition from a Dirac-like phase to a gapped phase. By comparing different multilayer structures we demonstrate that this transition occurs due to the hybridisation of states associated with different TI films. Our results demonstrate that the Sb2Te3-GeTe system offers strong potential towards manipulating topological states as well as towards controlledly inducing various topological phases.
Topological surface modes
Topological insulators (TIs) are a recently emerged class of materials which are insulating in the bulk, but whose surface harbours ‘topologically protected’ conducting modes1. The existence of the topological surface modes (TSMs) stems ultimately from the high spin-orbit coupling in TIs which ‘inverts’ the conduction and valence bands. In other words, the band structure of the TI is topologically distinct from the ordinary band insulator (BI) and the TSMs arise because the band gap must close at a TI-BI interface, or even an interface between a TI and the vacuum2. Importantly, local perturbations (e.g., disorder) which do not alter the topological properties of the system cannot localise the TSMs, and this gives rise to their ‘topological protection’. The TSMs have various exotic properties such as a linear Dirac-like dispersion, and a well-defined helicity, i.e., spin and momentum vectors at fixed angles to each other. These properties render them useful in a variety of settings such as low-power electronics and spin-based communication and computation. In addition, when TSMs couple to each other they are predicted to produce a very diverse phase diagram of novel topological phases3–5. In particular, in ref. 3 it was first proposed that superlattices of alternating TI and BI layers can overall either be TIs or BIs depending on the specifics of how the TSMs couple, and under certain conditions be Weyl semimetals6. Experimentally, there have been reports of TIs in superlattice structures including PbSe-Bi2Se3 structures7,8, Bi14Rh3I99, and Sb-Te binary systems10,11, although the crucial aspect of how the TSMs couple across the intervening layers remains unexplored. In this manuscript we investigate the low-temperature (low-T) electrical properties of molecular beam epitaxy (MBE)-grown bi-layer and tri-layer structures of Sb2Te3, a well-known TI12, and GeTe, a narrow band gap semiconductor that goes superconducting at very low T13,14. Intriguingly, our results indicate two-dimensional (2D) transport, indicating that the structures are dominated by the Sb2Te3-GeTe interface. Remarkably, we realise specific situations in which the tri-layer system has either a quadratically dispersive mode or three linearly dispersive Dirac-like modes. Based on very simple assumptions we argue that the two states are topologically distinct, thus suggesting Sb2Te3-GeTe heterostructures to be promising platforms to induce topological phase transitions and also realise multi-TSM systems3,4,15. TSMs in TIs have been most clearly identified using angle-resolved-photoemission-spectroscopy16,17, although this technique is unable to probe the interior of materials, and thus has limited applicability in studying buried 1
Cavendish Laboratory, Department of Physics, University of Cambridge, J. J. Thomson Avenue, Cambridge CB3 0HE, United Kingdom. 2Peter Grünberg Institute (PGI-9), Forschungszentrum Jülich, 52425 Jülich, Germany. Correspondence and requests for materials should be addressed to V.N. (email: [email protected]
Scientific Reports | 6:27716 | DOI: 10.1038/srep27716
Figure 1. The multilayer structures that are investigated are schematically depicted in (a). In (b) we show the T-dependence of ρ where, intriguingly, it is seen that the heterostructures have a lower ρ than both of the parent materials. (c) The carrier concentrations in the multilayers are more than an order of magnitude greater than that of pure Sb2Te3 and this is a direct outcome of the proximity to the larger bandgap material GeTe. (measurements from multiple samples are shown for D1 and T1). In (d) the data shown in (b) is plotted as a 2D resistivity ρxx. The right axis shows the measured resistance R. (e) Shows the ratio of ρxx in T1 and T2 to be ≈2.9, and that of D1 and T2 to be ≈2.5 at low T.
TSMs in structures of the type we report. Electrically, TSMs can be identified by observing quantum corrections to the conductivity σat low T. The strong spin-orbit interaction in TIs engenders positive quantum corrections to σin the form of weak antilocalization (WAL) at low T18 which manifests as a characteristic cusp in the magnetoresistance described by the Hikami-Larkin-Nagaoka (HLN) equation18: ∆σxx2D ≡ σxx2D (B⊥) − σxx2D (0) = α
1 e 2 + ln − Ψ 2 4eB⊥ 2ϕ 2π 2 4eB⊥ 2ϕ
Here σxx indicates the longitudinal component of conductivity and the superscript 2D indicates that the equation is valid for a two-dimensional conducting sheet, B⊥ is the magnetic field perpendicular to the 2D plane, αis a parameter = 0.5 for each 2D WAL channel, e is the electronic charge, is Planck’s constant divided by 2π, ϕ is the phase coherence length, and Ψis the digamma function. In TI thin films it is expected that α=1 due to the top and bottom surfaces, although often transport measurements in TI thin films are consistent with α ≈ 0.5, i.e., the existence of a single TSM19. There is a growing consensus that this is due to the interfacial disorder between the TI and substrate which destroys the bottom TSM. Importantly, this hinders progress towards understanding the interaction between TSMs. As an alternative, exfoliated TI structures have been used20 which are significantly less prone to interfacial disorder, but offer considerably less control over the film thickness. In this context, therefore, our approach of utilising MBE-grown multilayers is particularly promising in that it potentially overcomes both these limitations.
Results and Discussion
The wafer structures that we report here are schematically represented in Fig. 1a. The first is a double-layer structure with 11 nm of GeTe capped by 25 nm of Sb2Te3, henceforth referred to as D1. The second and third are three-layer Sb2Te3-GeTe-Sb2Te3 sandwich structures which we refer to as T1 and T2, respectively. In T1 each of the three layers is 15 nm thick, and T2 consists of a relatively thick 69 nm GeTe layer between 11 nm Sb2Te3 layers. The lattice mismatch of ≈2.5% between Sb2Te3 and GeTe is small enough to allow for coherent growth (see Methods). In addition, to benchmark our results, we have studied pure Sb2Te3 and GeTe films of thickness 48 nm and 34 nm, respectively. Figure 1b shows the resistivity P vs T of Hall bar devices fabricated from the different wafers. The first important fact to note is that, surprisingly, the multilayer structures are consistently less resistive than the pure samples, and closer in resistivity to Sb2Te3. Especially noteworthy in this context is that T2, which has the largest relative proportion of GeTe (≈76%), has the lowest ρ and shows the strongest deviation from pure GeTe. These observations clearly indicate that the individual layers do not behave simply as independent resistors connected in parallel, but rather interact with each other. One possibility is that the band bending at the interface between GeTe (band gap ≈ 0.65 eV21) and Sb2Te3 (band gap ≈ 0.2 eV22) serves to draw and confine additional charge carriers into Sb2Te3, and thus enhance its conductivity. This notion is corroborated by the measured areal carrier densities in D1, T1 and T2 being over an order of magnitude greater than in Sb2Te3 (Fig. 1c). Here we consider the areal rather than bulk carrier density since at low T the conduction in Sb2Te3 is largely through the Scientific Reports | 6:27716 | DOI: 10.1038/srep27716
Figure 2. (a–c) Show the WAL characteristics for D1, T1 and T2, respectively. Also shown are fits to the HLN formula (Equation 1). The traces are offset vertically for clarity. In (d) we observe that the rate of decoherence in T2 and Sb2Te3 is consistent with that expected due to inter-particle interactions, whereas in D1 and T1 the rate of decoherence is higher. (e) The parameter αwhich is a measure of the number of WAL channels contribute to the transport is seen to be 0.5 (corresponding to 1 WAL channel) for all the wafers except T2 in which αis approximately 1.5, suggesting the presence of three 2D WAL channels. (f) At low-T all the wafers show a logarithmic increase in ρxx as is expected in 2D systems. It is conceivable that in T1 and T2 GeTe is showing hints of superconductivity at ≈0.35 K, but this is unlikely to influence the transport unless T is reduced significantly.
TSMs and thus expected to be two-dimensional (2D)12. As a reference, the bulk carrier concentration in GeTe was measured to be ≈5 .5 × 1026 m−3 which, when scaled by the thickness of GeTe is ~1019 m−2, is comparable with D1, T1 and T2. In Fig. 1d we plot the 2D resistivity ρ xx ≡ ρ × t , where t is the thickness of the film, as a function of T: in order of increasing ρxx we find T2, followed by T1 and Sb2Te3 which are very similar below ≈1 00 K, followed by D1 and then GeTe. The strong dissimilarity between the characteristics of T1 and T2 suggests that there is more physics underlying the heterostructures than just band bending. We return to this fact after having inspected the low T electrical characteristics. 2 2 In Fig. 2a–c we show the low-field magnetoconductivity σ xx ≡ ρ xx /(ρxx + ρxy ) of D1, T1 and T2, respectively, and observe a pronounced cusp-like minimum around B⊥ = 0 T. Here ρxy is the Hall resistivity. The signal, e x p e c t e d l y, i s n o t c o n s i s t e nt w i t h b u l k WA L ( s e e S u p p l e m e nt a r y F i g u r e S 1 ) w h e r e ∆σ xx ≡ σ xx (B⊥) − σ xx (0) ~ B⊥1/2 23, but instead is very well-described by the HLN formula (Equation 1) with α and ϕ as fit parameters. We find that ϕ decays as a power law ~T−γ where the exponent γ is plotted in Fig. 2d. Apart from Sb2Te3 and T2, all the structures are observed to undergo decoherence significantly faster than the γ = 0.5 expected in 2D Nyquist scattering due to inter-particle interactions24. Figure 2e shows that α is ≈0.5 for Sb2Te3, T1 and D1, but is ≈1.5 for T2 (see Supplementary Figure S2 for error estimates on α). Recalling that α gets a contribution of 0.5 for each 2D WAL state, we conclude that Sb2Te3, T1 and D1 have one 2D mode each while T2 has three. While this is consistent with T2 being the least resistive sample under investigation (Fig. 1), there are two important points to consider: First, as discussed earlier in the manuscript, it is expected that α ≈ 0.5 for Sb2Te3 since the TSM at the substrate interface is destroyed. However, unexpectedly we find that even in D1, in which the Sb2Te3 film is grown on a well-lattice-matched MBE-grown GeTe film, a second TSM is not observed. Second, the occurrence of three 2D modes in T2 agrees with the three TI-BI interfaces (apart from the TI-substrate interface), but this is in apparent contradiction with the observation of only one 2D mode in T1. In a previous study it was found that bare GeTe thin films with t = 34 nm have α ≈ 114, i.e., one WAL mode on each side of the film, but GeTe has been intentionally omitted from this plot since it shows superconducting correlations below T ≈ 1.5 K which strongly influence the HLN fits14. In the following we investigate the precise role played by GeTe in these heterostructures. First, in order to check whether the tendency of GeTe to become superconducting at very low T has any influence on the transport properties of the multilayer structures we inspect the T-dependence of ρxx for T